ScientificDocumentationIPS e.max ® Ceram Page 8 of 21 3. Material science investigations 3.1 Comparative data with other veneering ceramics of Ivoclar Vivadent AG CTE 100-400°C [10 -6 K -1 ] IPS e.maxCeramIPS Eris for E2 9.50 ± 0.25 9.75 ± 0.25 Glass transition point Tg [°C] 490 ± 10 485 ± 10 Biaxial strength [MPa] 90 ± 10 85±25 Vickers hardness [MPa] 5400 ± 200 5600 ± 200 Chemical solubility [µg/cm 2 ] 15 ± 5 20 ± 10 Firing temperature[°C] 750 / 760 755 Type of material fluorapatite glass ceramic Amount of fluorapatite in the glass ceramic [% by wt] 19 – 23 28 - 48 Table 1: Comparative data with other veneering ceramics 3.2 Compatibility with IPS e.max materials 3.2.1 Coefficient of thermal expansion The linear thermal expansion of materials is measured with a dilatometer. A common way of measuring thermal expansion is by taking a length of material, heating/cooling it continuously and recording the resultant changes in length. This change in length may occur in a steady or discontinuous curve. A jump in the curve can be seen if a phase transition occurs in the material. The linear coefficient of thermal expansion (CTE) is determined per unit length for 1 degree change in temperature (1 Kelvin). The CTE largely depends on the temperature range within which it is measured. Hence, it is important to indicate the temperature range over which the CTE is determined, as the CTE alone does not have much informative value. The CTE of dental ceramics is determined within a temperature range that includes temperatures below the glass transition point (Tg). The CTE is utilized to identify potential stress levels that the ceramic may have to endure in conjunction with the framework and/or layering material. Glass ceramics at temperatures above the Tg value are soft and the stress is dissipated by the flow of the material. According to ISO 9693, the CTE is expressed in [10 -6 K -1 ]; the CTE is often also indicated as [1µm/m·K]. The coefficient of thermal expansion provides a clue as to whether the layering material is compatible with the framework material. Ceramic materials are very susceptible to tensile stress. As a consequence, the coefficient of thermal expansion (CTE) of the layering material should be lower than that of the more rigid framework material (Fig. 6).
ScientificDocumentationIPS e.max ® Ceram Page 9 of 21 CTE (100°-400°C) [10 -6 K -1 ] 11.5 11 10.5 10 9.5 9 8.5 8 IPS e.maxCeramIPS e.max ZirPress IPS e.max Press Fig. 6: CTE of IPS e.max materials (Ivoclar Vivadent Schaan, 2005) IPS e.max CAD IPS e.max ZirCAD � The CTE of the IPS e.maxCeram layering material is lower than that of the framework materials of the IPS e.max range. 3.2.2 Bond The bond between IPS e.maxCeram and the other IPS e.max materials can be clearly seen in the SEM images below. The “compo contrast" image has been produced with a special imaging technique: The different materials of the samples are depicted in various degrees of brightness in line with signal transmitted from the backscattering electrons (BSE). The signal is affected by the composition of the individual materials. IPS e.maxCeram forms a homogeneous, flawless bond with the materials of the IPS e.max range (Fig. 7 to Fig. 12). Fig. 7: Transition between IPS e.maxCeram (above) and IPS e.max ZirPress (below); (ground surface, etched) Fig. 8: Homogeneous, flawless bond between IPS e.maxCeram (above) and IPS e.max CAD; (“compo contrast”; polished surface)